This content has been downloaded from IOPscience. Please scroll down to see the full text.
IP Address: 22.214.171.124
This content was downloaded on 28/10/2014 at 09:52
Please note that terms and conditions apply.
Structural and optical properties of Zn-doped -Ga2O3 films
View the table of contents for this issue, or go to the journal homepage for more
2012 J. Semicond. 33 073003
Home Search Collections Journals About Contact us My IOPscience
Vol. 33, No. 7 Journal of Semiconductors July 2012
Structural and optical properties of Zn-doped -Ga2O3 films
Yue Wei(), Yan Jinliang(), Wu Jiangyan(), and Zhang Liying()
School of Physics, Ludong University, Yantai 264025, China
Abstract: Intrinsic -Ga2O3 and Zn-doped -Ga2O3 films were prepared using RF magnetron sputtering. Theeffects of the Zn doping and thermal annealing on the structural and optical properties are investigated. In compar-ison with the intrinsic -Ga2O3 films, the microstructure, optical transmittance, optical absorption, optical energygap, and photoluminescence of Zn-doped -Ga2O3 films change significantly. The post-annealed -Ga2O3 filmsare polycrystalline. After Zn doping, the crystallization deteriorates, the optical band gap shrinks, the transmittancedecreases and the UV, blue, and green emission bands are enhanced.
Key words: transparent conductive oxides; Zn-doped -Ga2O3; optical transmittance; optical band gap; photolu-minescence
DOI: 10.1088/1674-4926/33/7/073003 PACC: 7360F; 7855; 4225B
A need for ultraviolet transparent conductive oxide (UVTCO) films has recently emerged for use as antistatic electriclayers of the phase masks used for photolithography and astransparent electrodes for UV optoelectronic devices1; 2. De-velopment of UV TCO thin films is a challenge from amaterialscience point of view because materials with a wider band gaptend to exhibit smaller conductivity. Conventional TCOs suchas ZnO are opaque for the deep-UV light (< 300 nm) due to anarrow band gap (3.4 eV). New TCO materials need to be ex-plored in order to improve ultraviolet transparency. There areseveral difficulties in fabricating deep-UV transparent films.Since the position (scaled from the vacuum level) of the con-duction band bottom is relatively high, the donor levels tend tobecome deep levels. Introduction of the shallow donor levelsinto the compounds for efficient release of electrons into theconduction band is more difficult than in narrow gap oxides.This significantly reduces the number of candidate materialsfor deep-UV TCOs. -Ga2O3 is a wide band (4.8 eV) intrinsicinsulator36 and can be changed to n-type semiconductor bydoping7. It is suitable for the next generation of optoelectronicdevices operating at ultraviolet wavelength.
-Ga2O3 films with n-type conductivity up to 8.2 S/cmwere reported by Orita in 20021. Kiyoshi reported that thephotoluminescence of the -Ga2O3 could be improved by Sidoping8. The Si-doped -Ga2O3 and Sn-doped -Ga2O3 be-have as the n-type semiconductor because of donor impurityand oxygen deficiency9. To prepare -Ga2O3 based semi-conductor optoelectronic devices, P-type -Ga2O3 films areneeded. As one of group IIB elementsZn could be a potentialdopant for -Ga2O3. The radius of Zn2C is similar to Ga3C,thus Zn atom can substitute Ga atom efficiently. To the best ofour knowledge, few reports have been published on the struc-tural and optical properties of Zn-doped Ga2O3 thin films, es-pecially by means of magnetron sputtering.
In this article, the intrinsic Ga2O3 and Zn-doped Ga2O3films are prepared using RF magnetron sputtering, the effectsof the Zn doping and thermal annealing on the structural andoptical properties of the films are investigated.
The Zn-doped -Ga2O3 films (2 wt%) were deposited onSi (111) and UV transparent quartz (JGS1) substrates by RFmagnetron sputtering a Ga2O3 ceramic target at the power of70 W in a Ar/O2 (1 : 1) mixture atmosphere for 4 h. Before de-position, the quartz glass substrates were ultrasonically cleanedin acetone and alcohol, rinsed in deionized water and subse-quently dried in flowing nitrogen gas. The sputtering chamberwas evacuated to a base pressure of 6 104 Pa. The thick-ness of the films is about 320 nm. The films were prepared atroom temperature (RT) and then annealed in vacuum for 2 hat 800 C. The crystal orientation, photoluminescence, opticaltransmittance and optical absorption of the samples were char-acterized using X-ray diffraction (D/MAX2500V) with a Cu-K radiation source, a fluorescence spectrometer (RF-5301)and a double beam spectrophotometer (TU1901) by taking theglass substrates into consideration.
3. Results and discussion
3.1. Crystal structure
The XRD patterns of intrinsic -Ga2O3 films and Zn-doped -Ga2O3 films deposited on Si substrate and post-annealed in vacuum are shown in Fig. 1. Two predominantpeaks Si (111) and -Ga2O3 (111) are observed. It means thatthe post-annealed intrinsic -Ga2O3 and Zn-doped -Ga2O3films are polycrystalline and the Ga atoms are substituted bythe Zn atoms without changing the crystal structure. The inten-sity of the -Ga2O3 (111) peak becomes weak after Zn doping
* Project supported by the National Natural Science Foundation of China (No. 10974077), the Natural Science Foundation of ShandongProvince, China (No. 2009ZRB01702), and the Shandong Province Higher Educational Science and Technology Program, China (No.J10LA08).
Corresponding author. Email: firstname.lastname@example.orgReceived 1 January 2012, revised manuscript received 14 February 2012 c 2012 Chinese Institute of Electronics
J. Semicond. 2012, 33(7) Yue Wei et al.
Fig. 1. XRD patterns of intrinsic -Ga2O3 films and Zn-doped -Ga2O3 films deposited on a Si substrate and post-annealed in vacuumat 800 C for 2 h.
Fig. 2. Optical transmittance of as-deposited -Ga2O3 films and post-annealed -Ga2O3 films.
which indicates that the crystallization deteriorates. The posi-tion of the -Ga2O3 (111) peak shifts from 35.69 to 35.66because of the different radius of Zn2C and Ga3C (Zn2C:0.074 nm, Ga3C: 0.062 nm).
3.2. Optical properties
The optical transmittance of as-deposited -Ga2O3 filmsand post-annealed -Ga2O3 films is shown in Fig. 2. The as-deposited films show high transparency in the visible regionwith an average transmittance above 90% and an excellenttransmittance of more than 75% in the UV region (300400nm). Before annealing, the Zn-doped films have a slightly lowtransmittance. After annealing, the transmittance of Zn-dopedfilms decreases obviously in the UV and visible region. Itmeans the Zn dopant is activated by annealing.
The optical absorption of -Ga2O3 films before and af-ter annealing is shown in Fig. 3. All the films have a sharpabsorption edge in the deep UV region. Before annealing, theabsorption of the films increases after Zn doping. After anneal-ing, the absorption decreases obviously for the intrinsic filmsand increases for the Zn-doped films. The near-edge absorptionappears in the postannealed Zn-doped -Ga2O3 films, which
Fig. 3. Optical absorption of as-deposited -Ga2O3 films and post-annealed -Ga2O3 films.
indicates that the doped Zn atoms are activated effectively afterannealing and act as acceptors. Thus, the states of Zn acceptorsin the band gap of Zn-doped -Ga2O3 films should be respon-sible for the near-edge absorption. The near-edge absorptionrepresents transitions from singly ionized Zn acceptors to theconduction band bottom or from singly ionized Zn acceptorsto deep level donors such as oxygen vacancy (VO/ or intrin-sic defects10. The appearance of absorption of as-depositedZn-doped films means that the Zn dopant is not activated be-fore annealing, therefore, the increase of the absorption of post-annealed Zn-doped films should be mainly attributed to the ac-tivation of Zn dopant.
The optical band gaps of Zn-doped -Ga2O3 films are es-timated by extrapolating the linear portion of the square of ab-sorption coefficient against photon energy using Eq. (1).
.h/2 D A.h Eg/: (1)
HereA is a constant. Before annealing, the obtained opticalband gaps of the intrinsic-Ga2O3 and the Zn-doped-Ga2O3films are 4.90 eV and 4.87 eV, shown in Fig. 4(a). It indicatesthat the Zn dopant could reduce the forbidden band gap as aresult of lattice mismatch or stress. The optical band gaps of thepost-annealed intrinsic-Ga2O3 and Zn-doped-Ga2O3 filmsare 5.1 eV and 4.80 eV, shown in Fig. 4(b). As shown in Fig. 1,the crystallization of the intrinsic -Ga2O3 films is improvedafter annealing and some defect states in the forbidden bandare reduced, thus the optical band gap is expanded. For the Zn-doped -Ga2O3 films, the obvious change of the optical bandgap should be attributed to the efficient activation of the Zndopant which introduces the acceptor energy levels on the topof the valence band after annealing.
Room temperature photoluminescence (PL) spectra ofpost-annealed intrinsic-Ga2O3 films and Zn-doped-Ga2O3films are shown in Fig. 5, in which the green emission, the UVemission and the blue emission can be observed. The intensityof the emission systematically increases after Zn doping. Forintrinsic -Ga2O3 films, the UV emission and blue emissioncould be divided into four Gaussian peaks which are located at
J. Semicond. 2012, 33(7) Yue Wei et al.
Fig. 4. (a) Optical band gap of as-deposited intrinsic -Ga2O3 films and Zn-doped -Ga2O3 films. (b) Optical band gap of post-annealedintrinsic -Ga2O3 films and Zn-doped -Ga2O3 films.
Fig. 5. Photoluminescence spectra of (a) post-annealed intrinsic -Ga2O3 films and (b) Zn-doped -Ga2O3 films.
364 nm, 391 nm, 427 nm and 476 nm. At the same time, thegreen emission peak is located at 497 nm. The positions of thepeaks change slightly after Zn doping.
The UV emission could be attributed to the recombinationof self-trapped excitons11. Blue luminescence is associatedwith the recombination of a trapped electron in a donor witha trapped hole in an acceptor. Oxygen vacancies VXO or Gainterstitials GaXi are proposed as donors
12; 13. The gallium-oxygen vacancy pairs (VO, VGa/0 are proposed as acceptors.These donor-acceptor pairs can form trapped excitons result-ing in the blue emission according to the following process:.VO;VGa/X CVXO ! .VO;VGa/CV
O C h
13. Moreover, Znsubstituting Ga (ZnGa/0 should be another acceptor, so the blueluminescence is greatly enhanced when the (ZnGa/0 concentra-tion increases after Zn doping. The broad green band emissionwhich is located at 497 nm is generated by the radial recombi-nation of a photo-generated hole in VGa or VGa : VO and ZnGawith the electron in ionized VO.
The structural and optical properties of the intrinsic -Ga2O3 films and the Zn-doped -Ga2O3 films are discussed
before and after annealing. The transmittance of the as-deposited Zn-doped-Ga2O3 films is comparable to that of theas-deposited intrinsic films. The absorption of the as-depositedZn-doped-Ga2O3 films is higher than that of the as-depositedintrinsic ones. After annealing, both the intrinsic -Ga2O3films and the Zn-doped -Ga2O3 films are polycrystalline.The average absorption decreases for the intrinsic films andincreases significantly for the Zn-doped films. Three charac-teristic emission bands are observed, the UV emission and theblue emission are enhanced after Zn doping.
 Orita M, Hiramatsu H, Ohta H, et al. Preparation of highly con-ductive, deep ultraviolet transparent -Ga2O3 thin film at lowdeposition temperatures. Thin Solid Films, 2002, 411(1): 134
 Liu J J, Yan J L, Shi L, et al. Electrical and optical propertiesof deep ultraviolet transparent conductive Ga2O3/ITO films bymagnetron sputtering. Journal of Semiconductors, 2010, 31(10):103001
 Kim K S, Kim H W, Lee C M. Effect of growth temperature onZnO thin film deposited on SiO2 substrate. Mater Sci Eng B,2003, 98(2): 135
 Hajnal Z, Miro J, Kiss G, et al. Role of oxygen vacancy de-
J. Semicond. 2012, 33(7) Yue Wei et al.fect states in the n-type conduction of beta-Ga2O3. J Appl Phys,1999, 86(7): 3792
 Ueda N, Hosono H R, Kawazoe H. Anisotropy of electrical andoptical properties in -Ga2O3 single crystals. Appl Phys Lett,1997, 71(7): 933
 Kim H G, Kim W T. Optical properties of -Ga2O3 and -Ga2O3:Co thin films grown by spray pyrolysis. J Appl Phys,1987, 62(5): 2000
 Zhang J G, Xia C G, Deng Q. Growth and characterization ofnew transparent conductive oxides single crystals -Ga2O3:Sn.J Phys Chem Solids, 2006, 67(8): 1656
 Kiyoshi S, Encarnacion G, Vllora, et al. Excitation and photolu-minescence of pure and Si-doped -Ga2O3 single crystals. ApplPhys Lett, 2008, 92: 201914
 Suzuki N, Ohira S, TanakaM, et al. Fabrication and characteriza-tion of transparent conductive Sn-doped -Ga2O3 single crystal.Phys Status Solidi, 2007, 4(7): 2310
 Zhang Y J, Yan J L, Li Q S, et al. Optical and structural propertiesof Cu-doped -Ga2O3 films. Mater Sci Eng B, 2011, 176(11):846
 Harwig T, Kellendonk F, Slappendel S. The ultraviolet lumi-nescence of -gallium sesquioxide. J Phys Chem Solids, 1978,39(6): 675
 Harwig T, Kellendonk F. Some observations on the photolumi-nescence of doped -gallium sesquioxide. J Solid State Chem,1978, 24(3/4): 255
 Binet L, Gourier D. Origin of the blue luminescence of-Ga2O3.J Phys Chem Solids, 1998, 59(8): 1241